ELGEF Plus assembly instructions
The powerful electro-fusion system
for PE pressure pipelines
GEORG FISCHER 2
The technical data are not binding.They are not warranted characteristics andare subject to change.Please consult our General Conditions of Supply.
GEORG FISCHER 3
Assembly and operating instructionsELGEF Plus electrofusion fittings
Fundamental tipsElectrofusion for PE pipes and PE fittings enable safe, efficient and economical instal-lation of piping systems.Owing to the high quality standards of our products, tools and resources, the jointsare easy to make.
However, careful preparation of the fusion surface is the absolute prerequisiteand should not be neglected!
General tips for preparation and assembly of Georg Fischer fittings:Fusion zones should be well protected from moisture during inclement weather (rain,snowfall etc.).
Georg Fischer Fittings are supplied with the appropriate magnet card in a polythenebag. Fittings that arrive at the place of installation in their original packing, must nei-ther be machined nor cleaned with the PE cleaner. If the products (spigots) are never-theless machined, then it will not reduce the quality if it is done professionally. How-ever, it is not necessary.Exception: If the fusion zones are touched by hand during assembly, the fittings mustbe cleaned with the PE cleaner.
d Pipe Min. chip thickness Max. chip thickness*
2025 mm 0.20 mm 0.20 mm*3263 mm 0.20 mm 0.25 mm*75225 mm 0.20 mm 0.30 mm*> 225 mm 0.20 mm 0.35 mm*
Permissible minimum pipe outer diameter
d Pipe Min. chip thickness Per. minimum pipe outer diameter
20 mm 0.20 mm 19.6 mm 25 mm 0.20 mm 24.6 mm
32 mm 0.20 mm 31.5 mm 40 mm 0.20 mm 39.5 mm 50 mm 0.20 mm 49.5 mm 63 mm 0.20 mm 62.5 mm
75 mm 0.20 mm 74.4 mm 90 mm 0.20 mm 89.4 mm110 mm 0.20 mm 109.4 mm125 mm 0.20 mm 124.4 mm140 mm 0.20 mm 139.4 mm160 mm 0.20 mm 159.4 mm180 mm 0.20 mm 179.4 mm200 mm 0.20 mm 199.4 mm225 mm 0.20 mm 224.4 mm
250 mm 0.20 mm 249.3 mm280 mm 0.20 mm 279.3 mm315 mm 0.20 mm 314.3 mm355 mm 0.20 mm 354.3 mm400 mm 0.20 mm 399.3 mm450 mm 0.20 mm 449.3 mm500 mm 0.20 mm 499.3 mm
The pipe should be wiped, scraped and finally cleaned with the PE cleaner.Scraping tools should be used for even and time-saving pipe preparation.
The following scraping measurements should be maintained:
Tip: Maximum permissible pipe ovalness 1 .5%* the specifications refer to the pipe inner diameter without + tolerance
As a result: If the average pipe outer diameter is equal to the upper tolerance limit, the pipe can be cut outby scraping until the permissible pipe outer diameter. In this case, the chip thickness can be greater than 0.3 mm.
GEORG FISCHER 4
Use only PE cleaner with soft, absorbent paper to clean the fusion zones. Dusterssoaked in PE cleaner are allowed.
Clean only the scraped fusion surface. Otherwise, there is danger of tranferring dirt tothe already cleaned surface.
When using markers, check that no ink reaches the fusion zone. Even when cleaningmarker ink, take care that no ink touches the fusion zone.
Ink in the fusion zone cannot be removed completely despite repeated cleaning. Thepipe piece should be remachined or replaced.
Pipes that are oval or not round should be rounded using rounding clamps in theconnection zone.
Use brackets or suitable devices to fix the pipes and fittings. In particular when work-ing with roller pipes, ensure that no force is applied between the pipe and fusionzone during the fusion and cooling phase.
To transfer the fusion data to the fusion unit, you must always use the magnet cardand the barcode supplied in the original bag.
Wait until minimum cooling times before removing brackets, tapping and conductingthe pressure test.
Observe the assembly instructions.
RefusionIf there is power failure caused by external influences (for ex. generator failure) and if
The stability and surface hardness of PE 100 is greater than that of PE 80. This is es-pecially noticeable when the scraping tools become blunt. Therefore regular testingand maintenance of wear parts is required. We recommend servicing the units atleast once a year.
GEORG FISCHER 5
the electrofusion is subsequently interrupted, you can refuse the joint. The followingpoints should be kept in mind during refusion: Check and correct the cause of the fault. Appropriate error messages on the
fusion unit might provide tips on the possible cause. Do not remove the brackets. Cool the fitting completely again, i. e. cool to the ambient
temperature. Do not use other resources to cool the fitting (cold water etc.). Protect the joint from dirt and moisture during the cooling phase. Carry out the fusion again in accordance with the assembly instructions and
the specifications on the data carrier. Test the fusion for leaks, conduct a pressure test.
If the fusion joint fails in the pressure test, refusion is no longer possible.
GEORG FISCHER 6
Assembly instructions for sockets, fittings andadaptors
Sequence of tasks
7 Push in the PE pipe until the center stop or marking8 Firmly fasten integrated clamp9 Mount and fix assembly attachment
10 Slide in second pipe up to center stop or marking11 Firmly fasten integrated clamp12 Mount and fix assembly attachment
13 Follow operating instructionsfor fusion
1 Clean pipe(s), cut at right anglesand trim
2 Remove oxide film of pipe(s) usingscraper (adhere to max. permissiblewall thickness reduction)
3 Clean pipe(s) in fusion zone withduster and PE cleaner
4 Mark the insertion depth on thepipe
5 Remove the fitting(s) from thepackaging without touching thefusion surface.
6 Screw or unscrew transitionadaptor
16 Screw or unscrew transition-adaptor with loose clamping nut(if required)
17 Wait minimum waiting timeuntil pressure test, then conductpressure test
14 After fusion: Check fusionindicator on fitting and fusion unitdisplay, then remove cable15 Wait for cooling, finally remo-ve assembly attachment. Refer tomagnet card imprint and fusionunit display for cooling time
GEORG FISCHER 7
ELGEF Plus assembly instructions for sockets, fittings and transition adaptors
1 Clean pipe(s), cut at right angles and trim
2 Remove oxide film of pipe(s) using scraper
3 Clean pipe(s) in fusion zone with duster andPE cleaner
4 Mark the insertion depth on the pipe *1
5 Remove fitting(s) from the packaging without touching the fusion surface
6 Screw or unscrew transfer adaptor
7 Push in the PE pipe up to center stop or marking
11 Firmly fasten integrated bracket
10 Slide in second pipe up to center stop or marking
9 Mount and fix assembly attachment
8 Firmly fasten integrated bracket
12 Mount and fix assembly attachment
13 Fusion in accordance with operating instructions of the unit
14 After fusion: Check fusion indicator on fitting and fusionunit display, then remove cable
15 Wait for cooling, finally remove assembly attachment *2
16 Screw or unscrew transition adaptor with loose clampingnut (if required)
17 Wait minimum waiting time until pressure test,then conduct pressure test *2
*1 Insertion depth L1 in mm
d (mm) 20 25 32 40 50 63 75 90 110 125 140 160 180 200 225 250 280 315 355 400 450 500
L1 SDR 11 (mm) 34 34 36 40 44 48 55 62 72 79 84 90 97 104 112 112 112 112 122 122
L1 SDR 17 (mm) 95 100 105 110 123 135 123 123 123 145 145
*2 Minimum cooling time for sockets and fittings in minutes
d SDR Remove Pressure testbracket pl= 6 bar pl= 24 bar
(mm) (min) (min) (min)
20 63 11 6 10 30 75110 11 10 20 60125160 11 15 30 75180225 11 20 45 90250400 11 30 60 150450500
= compulsory = if required
Sequence of tasks
p = test pressure
SDR Remove Pressure testbracket pl= 6 bar pl= 24 bar
(min) (min) (min)
17 15 30 7517 20 45 9017 30 60 15017 40 60 150
GEORG FISCHER 8
11 Remove screw and fusion cap12 Tap clockwise, withdrawdrilling cutter up to the top stop;follow detailed assembly instruc-tions!
13 Fasten screw and fusion capby hand
14 Fusion in accordance withoperating instructions of unit
7 Align rotatable outlet and firmlyfasten integrated clamp of saddleoutlet
8 Fusion in accordance withoperating instructions of unit
9 After fusion: Check fusion indicatorof saddle; check fusion unit display,then remove cable10 Wait for minimum time untilpressure test, then conduct pressuretest
4 Place saddle on pipe andtighten with pre-mounted screws(stress clamp for strengtheningsaddle)
6 Place saddle on pipe andassemble with top-Load tool(detailed assembly instructions)
5 Remove modular system component from the packaging and assem-ble (without touching fusion surfaces)
Assembly instructions for saddles andtapping valves
Sequence of work
1 Clean pipe in fusion zone,remove oxide film of pipe usingscraper, (machine it, adhere tomax. permissible wall t